# Optimization of die-casting process parameters to ijiet.com/wp-content/uploads/2015/02/49.pdfOptimization of die-casting process ... optimization of Pressure die-casting process parameters

• View
217

5

Embed Size (px)

### Text of Optimization of die-casting process parameters to...

• Optimization of die-casting process parameters to identify optimized level for cycle time using

Department of Mechanical Engineering Late G. N. Sapkal COE, Nashik, Maharashtra, India

Shrikant V Karanjkar Department of Mechanical Engineering METs IOE, Nashik, Maharashtra, India

Abstract- This paper reports on an optimization of Pressure die-casting process parameters to identify optimized level for improving the cycle time using Taguchi method for DOE. AlSic132 up to 20tonn machine capacity is used to calculate cycle time. There are four machining parameters i.e. melting temperature, Injection pressure, Plunger speed, cooling phase. Different experiments are done based on this parameters. Taguchi orthogonal array is designed with three levels and four process Parameters with the help of software Minitab 15. In the first run nine experiments are performed and Cycle time is calculated. Taguchi method stresses the importance of studying the response variation using the signaltonoise (S/N) ratio, resulting in minimization of cycle time variation due to uncontrollable parameter. The Cycle time was considered as the quality characteristic with the concept of "the larger-the-better". The S/N ratio for the larger-the-better Where n is the number of measurements in a trial/row, in this case, n=1 and y is the measured value in a run/row. The S/N ratio values are calculated by taking into consideration with the help of software Minitab 15. The Cycle time values measured from the experiments and their optimum value for maximum cycle time. Every day scientists are developing new materials and for each new material, we need economical and efficient die-casting process. It is also predicted that Taguchi method is a good method for optimization of various Diecasing process parameters as it reduces the number of experiments. From the literature survey, it can be seen that there is no work done on AlSic 132 die-casting process. So in this project the Pressure die casting parameter of AlSic 132 is done in order to optimize the pressure die-casting process parameters for minimizing the Cycle time.

Keywords Taguchi Method, Die-casting Parameters, Pressure die-casting Process, AlSic 132, Software Minitab15.

I. INTRODUCTION

The die casting process involves the use of a furnace, metal, die casting machine, and die. The metal, typically a non-ferrous alloy such as aluminum or zinc, is melted in the furnace and then injected into the dies in the die casting machine.

There are two main types of die casting machines - hot chamber machines (used for alloys with low melting temperatures, such as zinc) and cold chamber machines (used for alloys with high melting temperatures, such as aluminum). The differences between these machines will be detailed in the sections on equipment and tooling. However, in both machines, after the molten metal is injected into the dies, it rapidly cools and solidifies into the final part, called the casting. Die casting equipment was invented in 1838 for the purpose of producing movable type for the printing industry. The first die casting-related patent was granted in 1849 for a small hand operated machine for the purpose of mechanized printing type production. In 1885, Otto Mergenthaler invented the linotype machine, an automated type casting device which became the prominent type of equipment in the publishing industry. Other applications grew rapidly, with die casting facilitating the growth of consumer goods and appliances by making affordable the production of intricate parts in high volumes. Die casting is a metal casting process that is characterized by forcing molten metal under high pressure into a mold cavity. The mold cavity is created using two hardened tool steel dies which have been machined into shape and work similarly to an injection mold during the process. Most die castings are from nonferrous metals, specifically zinc, copper, aluminum, magnesium, lead, alloys. Depending on the type of metal being cast, a hot- or cold-chamber machine is used. The Taguchi method is a well-known technique that provides a systematic and efficient methodology for process optimization and this is a powerful tool for the design of high quality systems. Taguchi approach to design of experiments in easy to adopt and apply for users with limited knowledge of statistics, hence gained wide popularity in the engineering and scientific community. This is an

International Journal of Innovations in Engineering and Technology (IJIET)

Volume 4 Issue 4 December 2014 365 ISSN: 2319 1058

• engineering methodology for obtaining product and process condition, which are minimally sensitive to the various causes of variation, and which produce high-quality products with low development and manufacturing costs. Signal to noise ratio and orthogonal array are two major tools used in robust design. The S/N ratio characteristics can be divided into three categories when the characteristic is continuous

a) Nominal is the best

b) Smaller the better

c) Larger is better characteristics

For the maximum material removal rate, the solution is Larger is better and S/N ratio is determined according to the following equation.

Where, S/N = Signal to Noise Ratio,

n = No. of Measurements,

y = Measured Value

The influence of each control factor can be more clearly presented with response graphs. Optimal cutting conditions of control factors can be very easily determined from S/N response graphs, too. Parameters design is the key step in Taguchi method to achieve reliable results without increasing the experimental costs.

AlSic132 is most suitable for the manufacture of parts such as Electrical enclosures, gear box, bolts and studs. AlSic132 withstand the highest operating temperatures of all the die cast alloys. Its strength, rigidity, and corrosive resistance offer significant heat dissipating. Aluminum is used in a broad range of networking and infrastructure equipment in the telecom and computing industries.

1.1 Processing Parameters that can affect process are

1.1.1 Melting temperature

The molten metal is poured into the die under pressure the temperature is measured in degree celsus.

1.1.2 Injection Pressure

Mould filling takes place while pouring the molten metal through the runner and gate and injection pressure is measured in Bar.

1.1.3 Plunger speed

Speed with respect to material is measured in m/s.

1.1.4 Cooling time

Finally, the mold is kept for cooling phase which is measured in Sec.

1.2 Equipment

There are two basic types of die casting machines: hot-chamber machines and cold-chamber machines. These are rated by how much clamping force they can apply. Typical ratings are between 400 and 4,000 st (2,500 and 25,400 kg).

1.2.1 Hot-chamber die casting

Hot Chamber Die Casting is the process where the injection system is immersed in pool of molten metal hence the name. The furnace is attached to the machine via a feeding system called a gooseneck. As the cycle begins the piston will retracts, which allows the molten metal to fill the gooseneck from a port in the injection cylinder. As the plunger move downwards, it seals the port and forces the molten metal through the gooseneck and nozzle into the die. Once the metal solidifies, the plunger will pull upwards. Afterwards, the die will open and the part is ejected. The advantage this process its short cycle time as it does not require metal to be transported from a separate furnace. Unfortunately, this die casting process is only suitable for alloys that do not attack the injection cylinder.

International Journal of Innovations in Engineering and Technology (IJIET)

Volume 4 Issue 4 December 2014 366 ISSN: 2319 1058

• Fig. 1.1 Hot-chamber die casting 1.2.2 Cold-chamber die casting

Cold Chamber Die Casting is the process of using a ladle to transport the molten metal from the holding furnace into the unheated shot chamber or injection cylinder. This metal is then shot into the die by using a hydraulic piston. However, this process is primarily used for manufacturing aluminum parts as molten aluminum alloys have a tendency to attack and erode the metal cylinders, plungers and dies greatly shortening their tool life.

Fig. 1.2. Cold-chamber die casting

II. OBJECTIVE

Select the component/s for study Identify the critical parameters for Processing the Cast components Capture the historical data for process parameters with its levels Perform DOE considering response factor as the cycle time or the quality of the component or any

suitable output parameter for the study Trial and testing upon development for experimentation Validate the thesis by comparing with the experimental results

2.1 Problem Definition

The sponsoring Company whose associate concern is primarily engaged in production of Die Casting is keen to investigate the levels for the factors responsible for arriving at the best quality for the cast components. Pressure die casting is primarily affected by the process parameters such as solidification time, molten temperature, Filling time, injection pressure and plunger velocity. It is therefore essential that the optimum casting technique with minimum defects be adopted to reduce the manufacturing cost of die casting component during mass production. The optimization of the process parameters pose a challenge for defects since the interplay among the parameters needs to be captured for setting the process for each component. In manufacturing processes, there are various parameters with different adjustment levels, which may influence the final characteristics of the product. To optimize a manufacturing pr

Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Engineering
Documents
Documents
Documents